| ||Format||Pages||Price|| |
|10||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||10||$48.00||  ADD TO CART|
Significance and Use
Corrosion testing by its very nature precludes complete standardization. This standard, rather than a standardized procedure, is presented as a guide so that some of the pitfalls of such testing may be avoided.
4.2 Experience has shown that all metals and alloys do not respond alike to the many factors that affect corrosion and that accelerated corrosion tests give indicative results only, or may even be entirely misleading. It is impractical to propose an inflexible standard laboratory corrosion testing procedure for general use, except for material qualification tests where standardization is required. One purpose for this guide is to promote better correlation of results in the future and the reduction of conflicting reports through a more detailed recording of meaningful factors and conditions.
4.3 In designing any corrosion test, consideration should be given to the various factors discussed in this guide, because these factors have been found to affect the results obtained.
1.1 This guide covers and describes the factors that influence laboratory immersion corrosion tests, particularly mass loss tests. These factors include apparatus, sampling, test specimen, test conditions (test solution composition, temperature, gas sparging, fluid motion, solution volume, method of supporting test specimens, duration of test), methods of cleaning test specimens, interpretation of results, and calculation of corrosion rates. This guide also emphasizes the importance of recording all pertinent data and provides a checklist for reporting test data.
1.2 The specific evaluation of localized attack, environmentally assisted cracking, and effects of solution flow are not within the scope of this guide.
1.3 This guide is intended to be used by those designing laboratory immersion tests who may not be familiar with all of the variables to consider and the pitfalls that could be encountered when designing and conducting this kind of testing. It should be used as a reference to ensure that the test will allow generation of data relevant to the application with the minimum of interferences.
1.4 The values stated in SI units are to be regarded as the standard. The values given in parentheses are for information only.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
ICS Number Code 77.060 (Corrosion of metals)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM NACE / ASTMG31-12a, Standard Guide for Laboratory Immersion Corrosion Testing of Metals, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top